1 Welding Procedure Specification (WPS) Code: AWS 1 of 3 Company Name: : 1 (877) WPS-WELDI dentification #: GMAW-DEMO WPS Prequalified:Yes Supporting PQR No.(s): N/A Welding Process: GMAWP rocess Type:Semi-AutomaticPosition(s):FlatBase Metal Part I (Material Spec., type or grade): Steels in Group I and II of Table Base Metal Part II (Material Spec., type or grade):Steels in Group I and II of Table Qualified Thickness and Diameter Range: Groove (Fillet): mm (in) T > = 6 mm (1/4 in) Filler Metals: AWS Classification/AWS Specification :E70C-6M H4 Joint Details/Sketch: Joint Design Used: mm (in) Root Opening G: 0 Root Face RF: > = 3 mm (1/8 in.) Groove Angle: 60 Radius (J-U): N/A Weld Type:Partial Joint Penetration Groove Weld Joint Type:Butt Joint Corner Joint Backing Option:Welded without backing Backing Material:N/A Back Gouging Method:N/A Identification #: GMAW-DEMOS heet 2 of 3 Electrical Characteristics:Current Type/Polarity:DCEPT ransfer Mode (GMAW):SprayTungsten Electrode (GTAW):Type: N/A Size: mm (in) N/A Shielding: Gas Composition (Flux for SAW): Ar + 5 to 15% CO2 Gas Flow Rate: lt/min.
2 (CFH) 40 to 50 CFH Gas Cup Size: 5/8 in. Welding ProcedureWeld LayersPass Filler Metal Classification Filler MetalDiametermm (in) Current Amps Current Type & Polarity Wire Feed Speed (in/min) Volts Travel Speed(in/min) Remarks[Heat Input]J/mm (J/in)1 1 GMAW E491C-6M-H4 mm ( ) 200-250 DCEP 200-250 25-27 10-14 Root Pass 1 to 2 2 to 3 GMAW E491C-6M-H4 mm ( ) 200-250 DCEP 200-250 25-27 10-14 Fill Pass 2 to n 3 to n GMAW E491C-6M-H4 mm ( ) 270-300 DCEP 270-320 26-28 12-18 Weld Size > =10 mm (3/8 in.) Technique: Stringer or Weave Bead: Stringer Bead Initial/Interpass Cleaning: Wire Brush, Grind Number of Electrodes: Single Electrodes Spacing: Longitudinal: N/A Lateral: N/A Contact Tube to Work Distance: 1 to1-1/8 in. Peening: N/A Angle: N/A Heat Treatment: Preheat Temp.
3 Min C ( F): 0 to 10 C-Table AWS Postweld Heat Treatment: Temp. C ( F): N/A Interpass Temp. Min/Max C ( F): 0 to 10 C-Table AWS Time: N/A Additional Notes:The end of contact tube recommended to be recessed in the cup nozzle at least 6 mm (1/4 in.) Manufacturer/ ContractorWelding Engineer: Name: Jim Clark Title: Welding Engineer Date: 12/12/2005 Authorized by: Name: John Smith Title: QA Manager Date: 12/12/2005 Identification #: GMAW-DEMO Sheet 3 of 3 Heat Treatment (AWS Code s Guideline): PREHEAT TABLE:Preheat and interpass temperature shall be sufficient to prevent cold need for and the temperature of preheat are dependent upon a number of factors such as chemical analysis, degree of restraint of the parts being joined, elevated temperaturemechanical properties, and material , Table Prequalified Minimum Preheat and Interpass Temperature F ( C):Preheat and Interpass temperature is provided for each material and thickness and process type on this material on Alternative Methods for Determining Preheat/Interpass.
4 See Annex XI of AWS requirements shall be based on Welding Procedure Specification (WPS). POSTWELD HEAT TREATMENT:PWHT requirements shall be based on Welding Procedure Specification (WPS).AWS , Stress-Relief Heat Treatment: Where required by the contract drawings or specifications, welded assemblies shall be stress relieved by heat treating. (See AWS , , Requirements for stress-relief treatment; Table , Minimum Holding Time; Table , Alternate Stress-Relief Heat Treatment)See AWS , , Steels Not Recommended for PWHT WPS Qualified Range (AWS Code s Guideline): Qualified Position (s): For Prequalified WPS, only Position (s) allowed for prequalified joint details shown inWPS based on Figures or of AWS Qualified Thicknesses: For Prequalified WPS, only thickness ranges allowed for prequalified joint detailsshown in WPS based on Figures or of AWS Qualified Diameters: For Prequalified WPS, pipe diameters [over or less than 24 in.]
5 (600 mm OD)] allowedfor prequalified joint details shown in WPS based on Figures or of AWS Prequalified WPS Base Metal Group Allowed: Only Base Metal Group-Filler Metal Combinations forMatching Strength as shown in Table of AWS Filler Metal Allowed in Prequalified WPS: Only Filler Metal-Base Metal Group Combinations for MatchingStrength as shown in Table of AWS (Size and other limit on electrode for prequalification of eachprocess, as per Table of AWS )